Presentation on theme: "Glenn Williams, Jeff Brum, Rachel Forcino, Fred Vogt GlaxoSmithKline XRPD Line Broadening Analyses to Study Micronization Induced Disorder and Environmental."— Presentation transcript:
Glenn Williams, Jeff Brum, Rachel Forcino, Fred Vogt GlaxoSmithKline XRPD Line Broadening Analyses to Study Micronization Induced Disorder and Environmental Annealing
Why Study Micronization Induced Disorder? Non-Micronized Milling Micronized Process of micronization results in significant attrition with consistent micron size particles, but the high energy process may also induce an element of “disorder” in the material. While this process improves dissolution and particle uniformity of the API the resulting “disorder” may affect stability and physicochemical properties, ultimately with a potential effect on dissolution and particle uniformity??
Changes in Physical Properties Are we investigating all the possible changes that may occur and the impact of those changes on the final formulation/processing and product? Surface Area Surface Energy Crystallinity XRPD Thermal DSC, TGA Moisture Sorp. GVS
Crystal “healing” or environmental “annealing” is often observed in aged/environmentally exposed materials Aging - API “hold times” Determination of the true contributions/components of disorder is necessary to understand and predict the effects on physicochemical properties and pharmaceutical processing
Micronized Ball milled Thermal Analysis Comparison of Milled API Tg Tg of amorphous standard higher than exotherm in micronized API
Surface vs Bulk Amorphous Wu, T.; Sun, Y.; Li, N.; de Villiers, M.; Yu, L. Langmuir 2007, 23, 5148 Lei Zhu & Janan Jona & Karthik Nagapudi & Tian Wu Pharm Res (2010) 27:1558–1567 Sayantan Chattoraj, Chandan Bhugra, Chitra Telang, Li Zhong and Zeren Wang, Changquan Calvin Sun. Pharm Res, 2012, Volume 29, Number 4, Pages
Amorphous griseofulvin 13 C T 1 and T 1ρ measurements Lower 13 C T 1ρ and T 1 values are consistent with higher molecular mobility in the ground sample Variable temperature measurements were not performed because of “ground” sample instability – recrystallization occurs rapidly under MAS spinning conditions 13 C T 1 13 C T 1ρ Melt-quench (initial) 1.60 ± 0.12 s78 ± 13 ms Melt-quench (ground) 0.74 ± 0.18 s45 ± 13 ms
Griseofulvin 13 C CP-TOSS spectra
13 C CP-TOSS spectra Micronized API(red trace) shows the signature of amorphous material
Micronized 60 psi Micronized 20 psi Thermal Analysis Comparison of API with Varied Micronization Energy Amorphous component (exotherm) increases with increased micronization energies
Gravimetric Vapor Sorption Re-crystallization
Post Gravimetric Vapor Sorption Post GVS After one GVS cycle the re-crystallization event is gone – consistent with amorphous recrystallization
Separating Components of Disorder Amorphous Thermal analysis GVS-recrystallization SS-NMR Nano-crystalline content XRPD – line broadening GVS/porosity Surface area
Why XRPD Line Broadening? Why study micronized materials by XRPD? Crystal is essentially a 3D molecular diffraction grating
The Scherrer Equation Peak width (B) is inversely proportional to the crystallite size (L) P. Scherrer, “Bestimmung der Grösse und der inneren Struktur von Kolloidteilchen mittels Röntgenstrahlen,” Nachr. Ges. Wiss. Göttingen 26 (1918) pp Short Range vs. Long Range Order
XRPD – Particle vs. Crystallite
XRPD – Instrumental Factors Same sample – Different instrument settings Need quality and consistent data collection
capillary Capillary sample may be loaded into holder (pre-aligned) and analyzed in standard transmission setup with auto-changer and without need for instrument reconfiguration to capillary analysis with standard goniometer heads. Convenient Capillary Analysis Setup Possible Spinning in both X-Y and X-Z planes XRPD – Sample Analysis
XRPD – Sample Analysis – Transmission Setup
Visual Comparison of Raw Patterns
Profile Fitting To Obtain FWHM FWHM
XRPD – Sample Analysis Non-micronized and freshly micronized materials show significant differences in linewidth – consistent and suitable for analysis
“Annealing” Studies Study 1 Samples of fresh micronized material were equilibrated at 6 different temperatures. Samples were heated in the DSC cell, in open DSC pans, and held isothermal for at least 60 min. Annealing 1. To subject (glass or metal) to a process of heating and slow cooling in order to toughen and reduce brittleness. 2. To strengthen or harden.
Study 1 Results Linear relationship observed with increasing temperature and XRPD linewidth (FWHM) – Increase in crystallite size as increase temperature
LiCl (~10 %)NaBr ( ~50 %)K 2 SO 4 (~95%) Ambient 50 °C Study 2 Samples of micronized material lot stored at 3 different RHs and at 2 different temperatures. Samples were pulled periodically over a several week period of time. Environmental “Annealing”
Study 2 – Time Course Within 2 weeks all conditions appear to have reached an equilibrium with respect to a reduced FWHM
Study 2 – Temperature Humidity Effect A synergistic effect on annealing is apparent with increased temperature and relative humidity
Freshly Micronized“Annealed” Microscope Comparison No obvious difference in particles post “annealing” - Consistent with healing of fractures/fines.
Healing of Fractures Increase in averaged crystallite size
Conclusions With further study we may be able to better understand “disorder” generated in micronized API’s and separate the contributions of true glassy amorphous and nano-crystalline content. We are currently evaluating the physiochemical changes that are associated with this observed crystal “healing” - related moisture sorption, surface area and porosity, thermal, XRPD, and ssNMR data. We are applying this same methodology to other projects with similar observations/results.
Acknowledgements Jeff Brum Rachel Forcino Fred Vogt (SS-NMR) Robert Carlton (SEM)